Originally approved in Last previous edition approved in as E–99 DOI: /E 2 For referenced ASTM standards. ASTM E()e1. Standard Practice for Microetching Metals and Alloys. standard by ASTM International, 06/01/ View all product details. Determination of Residual Stresses Numerically Obtained in ASTM AH36 Steel Welded by TIG Process. Pablo Batista Guimarães, Paulo.
|Published (Last):||28 June 2007|
|PDF File Size:||9.82 Mb|
|ePub File Size:||18.33 Mb|
|Price:||Free* [*Free Regsitration Required]|
Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If specimen has considerable surface?
Solutions are listed to highlight phases present in most major alloy systems. Mix in order given. Etching rate is increased, sensitivity decreased with increased percentage of HNO3. Distilled water may be added to maintain hydration, It must only be stored in plastic or glass bottles with nonmetallic 077. Gently agitate the solution while observing the polished surface. Will chemically polish with longer times.
[PDF] ASTM E Standard Practice for Microetching Metals and Alloys – Free Download PDF
Precaution—Keep cool when mixing and use. For etch-polishing, use awtm times. It may be helpful to place the specimen on a small piece of white paper.
Stains sigma and chi yellow to red brown, ferrite gray to blue gray, carbides barely touched, austenite not touched. Electrolytic at 3 V for 2—10 s. Electrolytic at 6 V: A superscript epsilon e indicates an editorial change qstm the last revision or reapproval. Immerse 1—2 s at a time and immediately rinse with methanol.
Swab for 5—60 s. Adding a wetting agent such as zepherin chloride will increase response.
Electrolytic at 15—50 V for 15—60 s. Where ethanol or methanol, or both are listed as alternates, ethanol is the preferred solvent. Pre-etch steel specimens with nital before tinting the MnS add 0. As cast Nickel Base: When more than one etchant number is given for a particular use, they are usually given in order of preference.
One or several small e4077 of a suitable dielectric compound with the desired index of refraction is heated under a vacuum until it evaporates.
ASTM E – 07()e1 Standard Practice for Microetching Metals and Alloys
Clean with cotton in running water. If that does not provide enough detailed information, contact the chemical manufacturer directly. Use stainless steel cathode and platinum or Nichrome connection to specimen. Some of these etchants will not work at all if water is not present. It will also react with alkaline materials including plaster and concrete to form explosive compounds. Continued Procedure Electrolytic in Solution A: Pure Co Hard-facing and tool metals High-temperature alloys 9, 10 11 12, 13c general structure via polarized light general structure general structure 14, 15, 16, 17 18, 19, 20 20, 18, 16, 21, 22b, 24, 25 19 general structure general structure general structure phase identi?
Immerse in Solution A for 2—5 s. Swab gently 5—15 s.
ASTM E407-07 Standard Practice for Microetching Metals and Alloys
Stop when surface is dark. Immerse 10—30 min depending on depth of worked metal layer. Electrolytic 5—10 V for 5—60 s. Etch time varies with material.
Follow with water rinse, alcohol rinse, dry. The specimen is placed in the solution using tongs, polished face up. Then electrolytic in Solution B: Composition Electrolytic at 2—3 V for 2—10 s.